- Email: [email protected]

Lattice Strain Mapping using Circular Hough Transform for Electron Diffraction Disk Detection Renliang Yuan , Jiong Zhang , Jian-Min Zuo PII: DOI: Reference:

S0304-3991(19)30167-6 https://doi.org/10.1016/j.ultramic.2019.112837 ULTRAM 112837

To appear in:

Ultramicroscopy

Received date: Revised date: Accepted date:

17 May 2019 22 August 2019 28 August 2019

Please cite this article as: Renliang Yuan , Jiong Zhang , Jian-Min Zuo , Lattice Strain Mapping using Circular Hough Transform for Electron Diffraction Disk Detection, Ultramicroscopy (2019), doi: https://doi.org/10.1016/j.ultramic.2019.112837

This is a PDF file of an article that has undergone enhancements after acceptance, such as the addition of a cover page and metadata, and formatting for readability, but it is not yet the definitive version of record. This version will undergo additional copyediting, typesetting and review before it is published in its final form, but we are providing this version to give early visibility of the article. Please note that, during the production process, errors may be discovered which could affect the content, and all legal disclaimers that apply to the journal pertain. © 2019 Published by Elsevier B.V.

Highlight

Electron nanodiffraction methods for determination of lattice strain are described and compared. A weighted 2D reciprocal lattice fitting method is proposed, including error analysis. Strain mapping resolution of 1 nm and precision of ~3×10‒4 is demonstrated on a Sibased FinFET device. An optimum strain mapping strategy is suggested based on experiments and simulations.

Lattice Strain Mapping using Circular Hough Transform for Electron Diffraction Disk Detection Renliang Yuana,b, Jiong Zhangc, Jian-Min Zuoa,b a

Department of Materials Science and Engineering, University of Illinois at Urbana-Champaign, Urbana, IL 61801, USA b Materials Research Laboratory, University of Illinois at Urbana-Champaign, Urbana, IL 61801, USA c Intel Corporation, Corporate Quality Network, Hillsboro, OR 97124, USA

Abstract Scanning Electron NanoDiffraction (SEND) is a powerful and versatile technique for lattice strain mapping in nano-devices and nano-materials. The measurement is based on Bragg diffraction from a local crystal volume. However, the resolution and precision of SEND are fundamentally limited by the uncertainty principle and scattering that govern electron diffraction. Here, we propose to measure lattice strain using a focused probe and circular Hough transform to locate the position of non-uniform diffraction disks. Methods for fitting a 2D lattice to the detected disks for strain calculation are described, including error analysis. We demonstrate our technique on a FinFET device for strain mapping at the spatial resolution of 1 nm and strain precision of . Using this and simulations, the experimental parameters involved in data acquisition and analysis are thoroughly investigated to construct an optimum strain mapping strategy using SEND. Keywords Electron diffraction; Semiconductor devices; Strain mapping; nanodiffraction; SEND analysis

1. Introduction Strain is an important structural property in materials science, as it impacts on many other physical properties. In semiconductor technologies, for example, strain is introduced to boost the performance of transistors by tuning the electronic band structure [1][2]. In metals and ceramics, inhomogeneous strain is introduced by defects or doping, and strain characterization is therefore critical to understanding materials mechanical, electronic and chemical properties. In transmission electron microscopy, strain is also a major source of image contrast [3] that has attracted continuous research interest [4][5][6][7][8]. In X-ray and neutron diffraction [9], the average strain is measured by diffraction peak broadening [10], although the recent trend is toward strain mapping using scanning [11]. Indirect measurement of strain can also be made using micro-Raman spectroscopy [12]. However, at the nm scale, transmission electron microscopy is the method of choice for high-resolution strain mapping. Electron beam based strain mapping can be performed in either imaging or diffraction mode. If the lattice fringes are resolved, strain can be calculated from electron images using the geometric phase analysis (GPA) method [4][5]. At atomic resolution, strain can be measured using GPA [13], or by analyzing individual atomic positions using the methods such as template matching analysis (TeMa) [14] or peak fitting [15]. Diffraction-based techniques measure the lattice dspacing in the reciprocal space using Bragg’s law. Lattice parameters can be determined at high precision from high-order Laue-zone (HOLZ) lines in convergent beam electron diffraction (CBED) [16][17]. In electron nanodiffraction (END) or nanobeam diffraction (NBD) using a parallel beam, lattice spacing is directly measured from the diffraction peak positions [18][19][20][21][22][23]. END describes all types of electron diffraction with a focused probe of nm size, which was first proposed by Cowley [24], while NBD is often associated with parallel beam diffraction [7]. The acronym SEND, adding the scanning aspect to END, was introduced in 2009 by Tao et al. [25], which was then further described in a book chapter in 2011 [26]. The END, NBD and SEND are versatile techniques as electron diffraction does not rely on highresolution imaging and can work with both thin and thick samples. Also, the strain measurement using diffraction also does not require the exact zone axis condition, as long as multiple diffracted beams are visible. This helps in dealing with sample bending, which is an issue in the samples with a large strain field. The detection of multiple diffracted beams can be further helped with precession electron diffraction (PED) [27]. In addition, diffraction patterns from different materials can be separated in the reciprocal space, which makes the characterization of complex device structures possible. The field of view (FOV) in SEND or NBD is determined by the scanning step size and number of steps used during acquisition [21][28]. The major challenge in the SEND or NBD based strain measurement comes from the uncertainty principle, as the spatial resolution ( ) and the peak width ( ) are coupled. In a SEND experiment on a thin sample, the spatial resolution is determined by the size of the focused electron probe, which is controlled by the beam convergence angle. In NBD, a near-parallel

illumination is often selected to produce sharp, and well-defined, diffraction spots using probes of several nm in diameter [18][19]. When the convergence angle is increased for higher spatial resolution, the diffraction peak is enlarged, which eventually becomes a disk as in CBED. The complicated contrast in a CBED disk due to diffraction presents a significant challenge to disk position detection, making strain measurement using CBED disks inaccurate [22]. To overcome this problem, Rouviere et al. [29] applied precession to the electron beam to reduce dynamic effects in the recorded diffraction patterns. Other efforts made to locate non-uniform diffraction disks include the radial gradient maximization method [20][30], template matching using crosscorrelation and its variations [21][31]. These methods improve the measurement precision, but still suffer from the detection error due to issues such as half-moon-shaped disks and the difference between the intensity of different diffraction orders, which limits the measurement accuracy. In this paper, we examine the entire procedure of strain mapping using SEND and propose a method for diffraction disk detection based on circular Hough transform (CHT). This method exploits the fact that although each diffraction disk has a different intensity distribution, their shapes are approximately similar, which is determined largely by the circular condenser aperture. The CHT can locate the center of a non-uniform diffraction disk even when a part of the disk edge is missing. Based on this, we develop a weighted 2D lattice fitting method to calculate the deformation matrix from the detected diffraction disk positions. The method is demonstrated through strain mapping on a 3D tri-gate FinFET device. An evaluation of the spatial resolution and strain accuracy and precision of our method is then presented based on the experimental result with the help of simulation, followed by suggestions on ways to achieve high resolution and high precision by optimizing the experimental parameters. In the end, we discuss and explain the effect of non-uniform strain field on the diffraction disk shape.

2. Methods 2.1 SEND data acquisition In SEND, a focused electron probe is rastered across a sample region of interest (ROI). Diffraction patterns are recorded at each probe position using a pixelated two-dimensional (2D) ) in detector. Thus, SEND collects a 4-D dataset, in the form of two spatial coordinates, the ( the real space and the ( ) in the reciprocal space. SEND can be done in either the transmission electron microscopy (TEM) mode using the TEM deflection coils [25][28], or in STEM mode [18][19][20][21]. When collecting the SEND data in a STEM, the HAADF detector can be used to record STEM images before, during, and after the acquisition to measure the sample drift and to apply drift correction accordingly. This is especially helpful when scanning a large area at a small step size as the entire acquisition could take hours to complete. Data acquisition is automated using either a dedicated hardware to synchronize the scan and diffraction pattern recording or by using computer control of the TEM and the electron camera. An implementation of SEND using the second approach is reported by Kim et al. [28]. The speed of acquisition is largely limited by the camera readout speed. For high precision strain mapping, the quality of electron diffraction patterns is critical in terms of the signal-to-noise ratio, the size

and the dynamic range of diffraction patterns. The impact of these factors on the measurement precision are discussed in Section 4. To evaluate the proposed 2D strain mapping method, we acquired a SEND dataset, taken from a source/drain region of a fin field effect transistor (FinFET). The TEM sample was a cut-out by focused-ion beam (FIB) from a p-MOSFET device processed with Intel 14 nm technology. The sample is about 30 to 40 nm in thickness and oriented near the [1-10] zone axis. The SEND data was acquired using a Themis Z S/TEM (Thermo Scientific, Waltham, USA), installed at University of Illinois, which was operated in the Probe STEM mode with the acceleration voltage of 300 kV. The electron probe was focused on the sample with a semi-convergence angle of 0.8 mrad, and the probe size of 1.0 nm in FWHM. Camera length was set at 360 mm where all 8 diffraction peaks adjacent to the center beam in the [1-10] zone axis were included in the recorded image. Diffraction patterns were taken using a CMOS camera (Ceta, Thermo Scientific ) at the resolution of 1024x1024 pixels and 0.1 s exposure time per diffraction pattern. No pixel binning was applied. The scanning and diffraction data acquisition were automated by a function in the TEM control software provided by Thermo Scientific. During the scan, a new STEM image, containing the scanned region, was acquired by the HAADF (high-angle annular darkfield) detector every 60 frames for sample drift correction. Additionally, the sample was observed using ADF STEM images, which were acquired using the same electron probe and camera length setting as for SEND. The ADF detector collection angle is 16-96 mrad, and the recorded STEM images contain information from both Z-contrast and diffraction contrast.

2.2. Diffraction disk detection using circular Hough transform After a SEND dataset is recorded, the first step is to reduce the 2D diffraction pattern into a list of diffracted beam positions. Several image processing techniques can be employed for this purpose based on the feature in the diffracted beam. In NBD using a parallel beam illumination, the diffracted beams are recorded as sharp diffraction spots. Locating the peak position, in this case, can be done by using a 2D peak searching and fitting algorithm. Under the convergentbeam condition in SEND, however, the diffracted beams become disks. In this case, the template matching method (TMM) using cross-correlation has been used to transform the disks into correlation peaks in the calculated correlation map [21]. Another method is to use edge detection and CHT to reduce diffraction disks into sharp spots [32]. In what follows, we describe the details of the CHT based diffraction disk detection technique.

2.2.1. Circular Hough transform In the theory of high energy electron diffraction from a periodic crystal, the only similarity among the diffraction disks is the shape of the disk, resembling the approximate circular shape of the condenser aperture. Within the diffraction disks, varying rocking curve features are recorded, which depend sensitively on the crystal orientation and thickness, which presents a significant challenge for the accurate measurement of the diffracted disk position. To overcome this challenge, we propose an edge-based detection method to locate the diffraction disks. At the core of this method is CHT [33][34]. As illustrated in Fig. 1a, all points on a circle, as specified by

), are transformed into circles in the so-called accumulator matrix of their coordinate ( ), satisfying the equation ( coordinates ( ) ( ) , where is the radius of ) point is the center of one circle. After accumulating all circles, the the circle. Here, each ( ) of the original circle, ( point where the circles intersect is exactly at the center ( ) ( ) . In the pixelated accumulator matrix at the same resolution as the original image, each pixel counts the number of circles passing through it. When the exact value of the radius is unknown, an estimated range of radius is used to generate the accumulator matrix. After CHT, the problem of disk detection is simplified to 2D peak finding in the accumulator matrix.

Fig. 1. Diffraction disk detection using CHT. (a) A schematic illustration of CHT, where points on the original circle are transformed into circles in the accumulator matrix, the center is defined by the intersection of the transformed circles. (b) An example of experimental diffraction disk is edge-filtered (c) and then transformed using CHT (d). (e) The disk center is determined by fitting the horizontal and vertical projections of the accumulator matrix using Lorentzian peak fitting. The center identified by this method is marked by a red crosshair in (d).

The procedure of detecting diffraction disks using CHT is summarized in Figs. 1b-e. First, a Sobel filter: (

),

(1)

and its transpose are used to obtain the gradients in horizontal and vertical directions, X and Y. Combined together, is the filtered edge as shown in Fig. 1c. Next, the edge is transformed into an accumulator matrix using CHT. An estimated radii range of pixels around the exact radius is applied to provide sufficient sampling to represent the transformed peak. The transformed peak is then projected both vertically and horizontally to allow for 1D peak fitting as described in Section 2.2.2. The fitted peak positions are taken as the coordinates of the diffraction disk center ( ). As shown in Fig. 1c, information inside the disk is mostly discarded by the Sobel filter. The CHT works well even when parts of the edge are missing. The detection is sensitive to the intensity of a few edge pixels. The width of the edge reflects the sharpness of the disks. This fact also makes the combined edge detection and CHT method sensitive to intensity noises. Section 4 gives a detailed discussion on this issue. 2.2.2. Peak fitting To detect the position of a CHT peak, we use the peak fitting method. The peak finding method can also be applied directly to spot diffraction patterns. The method we describe here is based on 1D peak fitting to the projected peak intensity profiles (line profiles) in horizontal and vertical directions, respectively. First, a sub-image containing only the peak of interest is cropped out. The sub-image is then projected horizontally and vertically to produce two line-profiles. For the peak model, depending on the peak shape, we use the Lorentzian profile: (

)

((

)

,

)

(2)

where is peak position, and is half-width at half-maximum. The peak model is fitted to the line profiles to extract the horizontal and vertical positions of the diffraction peak ( ). Error analysis can be performed as part of the fitting.

2.3. Diffraction disk detection using template matching The image processing technique described below based on template matching can be used to transform the disks into spots for peak fitting. This method, which was proposed before [31], will be compared with the CHT method in this paper.

Template matching works by comparing the targeted image of size with a template image of size ( ) to find the best match between and a sub-image ( ), where ( ) is the position of the sub-image in . The way to do so is by calculating correlation coefficient between and ( ) for and : (

)

∑ [ ( √∑ [ (

(̅

) )

)][ ( (̅

)] √

) ̅]

,

(3)

where the summation runs over all and j . (̅ ) and ̅ are average value of image ( ) and . is the total number of pixels in . is the variance of . In addition to Eq. 3, several other definitions of correlation exist [31]. Fig. 2 shows an example of template matching for an END pattern (Fig. 2a). A template (Fig. 2b inset) was obtained by cropping out a relatively uniform center disk. Using this template, the END pattern in Fig. 2a is transformed into correlation peaks, which can be measured using the peak fitting method from Section 2.2.2. The TMM works best when the diffracted beams recorded in diffraction pattern are similar. The assumption that all disks are similar is approximately valid only in kinematical CBED (KCBED) [35]. The intensities within a given diffraction disk can also be made uniform by using PED [27]. To reduce the diffraction collection time, a setup of PED using a fast precession control unit is also required. For CBED patterns recorded without precession, the variations of rocking curve intensities are the major sources of error for strain analysis using template matching.

Fig. 2. Diffraction disk detection using template matching (TMM). (a) Example diffraction pattern. (b) Correlation map calculated using the template image in inset.

2.4. Determining the two-dimensional (2D) reciprocal lattice

Fig. 3. Schematic of measuring the reciprocal basis vectors ⃗⃗⃗⃗ and ⃗⃗⃗⃗ from a diffraction pattern by fitting a 2D lattice to the position of the detected disks.

In a diffraction pattern taken at or near a zone-axis, diffraction peaks lie on a 2D grid defined by the reciprocal basis vectors ⃗⃗⃗⃗ and ⃗⃗⃗⃗ , and the center position ⃗ (Fig. 3). The measured diffraction peak position gives ⃗⃗⃗ . A fitting to the measured peak positions is carried out to determine ( ⃗ ⃗⃗⃗⃗ ⃗⃗⃗⃗ ), where ⃗⃗⃗

⃗⃗⃗⃗⃗⃗⃗⃗

,

(4)

⃗⃗⃗⃗⃗⃗⃗⃗ ⃗ Here ⃗⃗⃗⃗ ⃗⃗⃗⃗ ( and are integers) and represents error. The best fit is obtained when the distance between the measured and the fitted peak position is minimized with respect to the measurement error. To meet this requirement, we define a weighted residual sum of squares ∑ (

)

(

) , (5)

where ( ), ( ) are the horizontal and vertical components of the measured and fitted positions of the peak, respectively. and are the standard deviation in the measured peak position, which are used as a weight to increase the contribution from those well-measured peaks. Calculation of and is detailed in next section. If and are both set to 1, no weight is applied, and Eq. 5 becomes the sum of squares of the distance between measured and fitted peak position. The summation runs over all detected peaks in the image. Written in the matrix form, we have (

) (

)

where

(

, (

)

(

) (

(7)

)

, (

)

),

(

)

(8)

(6)

(

)

(

). (9)

The minimum is achieved when {

(

)

(

)

.

, which gives

(10)

The above solution is used to set up the reciprocal lattice matrix

(

)

2.5. Estimate of measurement precision Error in the peak position can be estimated using the 0.95 confidence interval of the peak fitting: √ ,

(11)

where is the fitted peak position, is the error in peak position. is a constant dependent on the confidence level and the degree of freedom, which can be calculated from Student’s distribution. when degree of freedom is large at 0.95 confidence level. is the covariance matrix of the coefficient estimates: (

)

,

(12)

where is the Jacobian of the fitted values with respect to the coefficients and squared error.

the mean

According to Eq. 10, error in refined reciprocal lattice vectors can be calculated as ( )

(

where

)

( ) ((

)

) , (13)

.

Error in ( )

vector along any reciprocal direction ( (

)

( ) ( ).

Finally, error in strain along (

( ))

(

⃗⃗⃗⃗

⃗⃗⃗⃗

(14)

is )

( ).

(15)

) is

2.6. Calculation of the strain tensor Based on the reciprocal lattice matrix and a reference matrix , the real space lattice matrix and its reference , and local deformation matrix in Lagrange convention can be calculated: (

)

.

(16)

For the general case without infinitesimal approximation, the deformation matrix (

) can be separated into a rotation matrix

and a pure deformation matrix

through

polar decomposition. [5] Following the derivations in Ref. [5], rotation angle

(

). Pure deformation is a

symmetric matrix: (

) .

(17)

The local 2D strain tensor can be expressed as the difference between (

)

.

and unit matrix:

(18)

2.7. Diffraction pattern simulations To help interpret our experimental results, we use the multislice method to simulate electron nanodiffraction using a modified version of the MULTIS program published in [36]. For the simulation, the electron probe is assumed to be fully coherent and is formed by Fourier transform of the aperture function without aberrations. A supercell of 40 nm by 40 nm in dimensions and 4096 by 4096 in sampling points is constructed to model the sample using the atomic scattering potential with the absorption due to the effect of phonon scattering included. The probe is then scanned across the supercell and its diffraction pattern is recorded at each probe position.

3. Application

Fig. 4. Strain mapping of a Si-based FinFET device. (a) Medium-angle (16-96 mrad) annular dark-field image of the scanned region taken by an ADF detector with the same condition for strain mapping, which is used for drift correction during scanning. (b) Reconstructed virtual bright-field image of the scanned region shows that sample drift is well compensated. Maps of (c) , (d) , (e) , and (f) rotation calculated from the scanning diffraction dataset at 1 nm spatial resolution. The image dimension is nm2. Vertical dashed lines in (b) and horizontal dash-dotted lines denote the position of strain profiles shown in Fig. 7a and Fig. 11a, respectively. The black arrows mark the probe position where diffraction disks in Figs. 11b and c are taken. The white arrows in (c-f) mark the increasing (pointing right) and decreasing (pointing left) strain and rotation. The maximum strain is smaller than the difference between the lattice constants of pure Si and Ge, which is 4%. The exact values are not shown in accordance with Intel’s regulation.

Fig. 4 shows the results of 2D strain mapping on the source/drain area of a FinFET. The SEND map size is 60 by 120 pixels with the pixel (step) size of 1 nm. The designated scan area is shown in Fig. 4a, which is a ADF-STEM image taken at the beginning of the SEND experiment. Additional STEM images were also acquired during the SEND acquisition, which are used for drift correction based on the sharp features in the image for sample registration. Fig. 4b shows a virtual bright-field (VBF) image, reconstructed from the SEND dataset by integrating the intensity in the center disks. The good correspondence between the ADF-STEM image and the VBF image, apart from the inverse contrast, indicates that the sample drift during acquisition was well-compensated using our drift correction procedure. Figs. 4c-f display the strain maps of longitudinal and , shear , and rotation , which are obtained following the methods described in Section 2. The diffraction disk positions were detected using the CHT method and the CHT peak fitting by the Lorentzian profile. The 8 loworder diffracted beams and the center disk as shown in Fig. 3 were used to refine the reciprocal lattice matrix G, where the (111) disk was designated as ⃗⃗⃗⃗ and the (11-1) disk as ⃗⃗⃗⃗ (Fig. 3). The strain tensor was calculated based on the averaged reference matrix from a flat substrate region near the bottom of the scanned area.

The direction in Figs. 4c-f is defined as the [110] direction of the reference lattice, and the direction is [001]. Strain map shows clearly the interface between SiGe and Si substrate, marked by yellow arrow in Fig. 4c, as can also be seen in ADF-STEM or VBF images, while it is not visible in , reflecting the epitaxial nature of strain. The maximum of strain in both and is reached at the top of source/drain where it is attached to metal contact. The crystal shear and rotation are also most severe in this region. Another interesting feature in Fig. 4 is that the map appears noisier than the map, meaning that the precision in measurement is lower. This is correlated with the shorter length of (002) compared with that of (220). Assuming that the disk detection error is similar for the two cases, the strain error is larger where the length of g is shorter. Further discussion on the precision can be found in Section 4.4. 4. Discussion 4.1. Spatial resolution of SEND based strain mapping

Fig. 5. Relation between the electron probe size and beam semi-convergence angle at 300kV. The probe size is measured by the full width at half maximum (FWHM).

The spatial resolution of strain mapping using SEND can be taken approximately as the electron probe size or the column diameter √ , whichever is larger [28]. The electron probe is diffraction limited according to Rayleigh criterion , for a small convergence angle. For a given acceleration voltage, the electron probe size decreases as the convergence angle increases, which then stabilizes because of aberrations, as can be seen in Fig. 5. In high-resolution STEM, the beam convergence angle is much larger at ~10 to 30 mrad. The large convergence angle is used to form Å or sub-Å sized electron probes. For strain analysis using SEND, however, the convergence angle is kept small so that neighboring diffraction disks do not overlap, as the overlapping disks make disk detection imprecise. At the limit where the disks touch each other, the probe size is about the size of d-spacing, which is the limit for strain mapping since strain is defined at the lattice level in most applications. The measurement precision improves as the volume of crystal for diffraction increases. Because of this, a nm-sized electron probe is preferred over the smaller, sub-nm sized, probes. The same correlation between the spatial resolution and the precision of strain measurement is also found in the real-space based strain mapping techniques [14].

4.2. Impact of sample orientation and thickness on the strain measurement accuracy

Fig. 6. Comparison between accuracy of template matching (TMM) method and circular Hough transform (CHT) method based on multislice simulation of unstrained/strained Si model structure. Error in strain along [110] direction of using the (a) CHT or (b) TMM method to detect diffraction disks from a sample of 8 nm thick. Different intensity distribution in the disks is achieved by tilting electron beam around x || [110] direction and y || [001] direction. (c) Comparison of strain measurement error on single crystal sample between two methods along 110 and 001 directions at various sample thickness. Each data point is an average of a tilt series of 25 patterns. (d) Comparison of strain measurement error on sample strained along [110] direction. Each data point is an average of 10 different probe positions and 25 beam-tilt combinations, totaling 250 patterns.

Real samples are often bent and have varying thicknesses, the error caused by change in the diffraction condition is systematic that limits the strain measurement accuracy. Here, we examine the strain measurement accuracy as impacted by variations in the sample orientation and thickness with the help of simulation. We compare the intensity-based method (TMM) with the edge-based method (CHT) based on the simulated SEND patterns. The model we used to test the methods is a perfect Si crystal oriented along the [1-10] zone-axis. Electron diffraction was simulated using the multislice method as described in Section 2.7. The first set of simulations tilted the beam around the zone axis from 0.1 to 0.4 along the x || [110] and y || [001] directions for a sample of 8 nm in thickness. Since there is no strain built in the model and the distances between the diffraction disks in the simulated diffraction patterns are

determined by the reciprocal lattice vectors, any measured strain (change in the measured dspacing) can be attributed to the error of the diffraction disk detection method due to change in diffraction intensity, which we simply refer as strain error. Figs. 6a and b display the strain error from the simulated diffraction patterns using the CHT and TMM, respectively. Comparison between these two figures shows that while the strain error in TMM is strongly correlated with the beam tilt, the error in the CHT method is much less. We then repeated the simulation with the sample thickness by varying the simulation thickness from 8 nm to 80 nm. Fig. 6c plots the strain error from these simulations. Each data point in the plot is an average of 25 strain values measured from 25 simulated patterns of different beam tilt following the same routine in Figs. 6a and b. The above results show that the edge-based detection method tends to have a higher accuracy than the intensity-based method when it comes to detecting non-uniform diffraction disks. The CHT method is relatively insensitive to the intensity changes due to sample bending and variations in sample thickness. Especially when the sample is thick and the intensity pattern is complicated, the strain error using CHT is kept below 0.05%, which is far better than the performance of TMM. 4.3. Strain measurement accuracy of a sinusoidal strain field Next, we test our methods using an artificial strain model by displacing atoms from their original positions in the model Si structure along the [110] direction. The strain field we introduced is sinusoidal with the amplitude of displacement at 1% over the period of 80 unit cells. The electron probe was scanned over the area where the strain changes from -1% to 1%. Overall, 10 different strain values and different local strain gradients are sampled here. At each probe position, 25 beam tilts as in the unstrained case of previous section were simulated. The strain error was averaged over 250 simulated patterns. The results are plotted vs sample thickness in Fig. 6d. The error using the CHT method is less than 0.1% for sample thicknesses up to 80 nm. The difference between Fig. 6d and Fig. 6c is attributed to the effect of local strain variation on electron diffraction. The volume illuminated by the electron beam is no longer a perfect lattice here. Thus, the diffraction patterns of different beam tilt come from differently strained regions, and the variations in the sample orientation and thickness cause fluctuations in the measured strain, which reduces the accuracy of the CHT method. Deviation due to a finite-sized probe will be further discussed in Section 4.6. 4.4. Strain measurement precision In this section, we evaluate the precision of strain measurement using two different methods. One is by performing a calibration experiment on an unstrained crystal. The other is through error analysis based on the fitting error of diffraction disks as described in Section 2.5. The error analysis method can be applied directly to the experimental dataset. Both methods provide an assessment of the measurement precision or sensitivity. As electron diffraction from a strained crystal is different from that of an unstrained crystal, the measurement precision is also sample dependent. In applications, the 3D nature of sample strain is often unknown. Because of this, we

prefer to discuss the measurement precision rather than the measurement accuracy, which is discussed in the previous section for a known strain model. The calibration experiment was carried out on a flat region of Si substrate in the FinFET device measured in Section 3, using the same experimental condition as in Fig. 4. The scanned area was selected to be close to the strained source/drain region in Fig. 4 so the sample thicknesses in the two measurements are similar (~40 nm). The scan size is 10 by 10 pixels with a step size of 1 nm. The measured strain value is plotted in Fig. 7 along with the strain profiles extracted from the 2D strain maps in Fig. 4. The standard deviation obtained from the calibration scan can be taken as the strain measurement precision, which is 0.036% along the [110] direction and 0.076% along the [001] direction, respectively. The difference in the strain measurement precision along two different directions explains that the difference in smoothness seen in Figs. 4c and d, where Fig. 4c appears smoother than Fig. 4d. The smoothness reflects the measurement precision.

Fig. 7. Example strain profiles from strained and unstrained regions of a FinFET transistor. (a) Profiles of strain along [110] and along [001] extracted from the strain maps in Figs. 4c and d. (b) Profiles of and measured from a relatively uniform substrate region for calibration.

The calibration experiment was performed on a single crystal region. Thus, it does not capture the diffraction features from a strain field. Because of this, it tends to underestimate the error in real experiments on a strained lattice.

The strain measurement precision can be estimated directly from the acquired SEND data via an error analysis based on the fitting error of each diffraction peak. From the description in Section 2, in both TMM and CHT, the peak position is determined by peak fitting. We calculated the error maps for the strain maps and using the method described in Section 2.5, the results are shown in Fig. 8. From the error maps, we can see that strain precision is lower at the interfaces, especially near the bright edge at the top of both maps where the crystalline structure meets the amorphous film. The average error excluding the interfacial region at the top is 0.029% and 0.075% along the [110] and [001] directions, respectively. This agrees with the trend that the strain along [110] can be measured at a higher precision than along [001] as observed in the Si substrate calibration experiment.

Fig. 8. The calculated error maps for strain (a)

and (b)

on the FinFET device.

4.5. Optimize the experimental conditions for higher precision

Fig. 9. Diffraction disk detection error using CHT at different signal-to-noise ratios.

The strain measurement precision is determined by the precision of disk detection, which can be improved by optimizing the experimental conditions, including the diffraction intensity level and noise, the diffraction camera length and the beam convergence angle. The diffraction intensity level and noise in an acquired diffraction pattern is measured by the signal-to-noise ratio (SNR), which is a critical parameter. Here we define the SNR of a diffraction disk as ̅̅̅̅̅̅̅

, (19)

where ̅̅̅̅̅̅ is the average intensity in a diffraction disk, and the background intensity.

is the standard deviation of

To examine the effect of SNR on disk detection, we performed a calibration experiment in vacuum (without sample) using the same electron probe for the strain measurement described in Section 2. The experiment was done without scanning to avoid the scan noise. The SNR was controlled by changing the electron beam intensity using mono-focus in the Themis Z STEM. At each SNR level, 100 diffraction patterns were acquired. The recorded diffraction patterns contain a single flat disk that differ in intensity and in noise (including the electron beam noise due to the instrument and environmental instabilities). The error in the detected disk position is calculated from the standard deviation of the measured disk positions in the acquired patterns. The result of

using CHT to detect the disk is shown in Fig. 9. The detection error is inversely proportional to SNR. The proportionality can be attributed to the effect of noise on the disk edges, which become less defined as noise increases, leading to larger errors in disk detection. The error decreases as the SNR increases, and the improvement slows down when , which can be taken as a cutoff for acquiring a good diffraction dataset for the strain measurement using CHT.

Fig. 10. Diffraction disk detection error using CHT for different disk radius. (a) An example of the measured disk position x from 100 patterns recorded over vacuum using CHT and TMM and their difference. Error in diffraction disk detection using CHT for different disk size achieved by changing (b) the camera length and (c) the convergence angle.

Another deciding factor for disk detection is the disk size, which is determined by the camera length as well as the convergence angle. Figs. 10b and c show the relation between the disk

detection error and the disk radius. Following the same procedure as in Fig. 9, the plotted detection error here was calculated from the standard deviation of the detected disk position from 100 exposures in vacuum using the CHT method, while the SNR was kept same for all disk radii. The fluctuation in the detected disk position came from the error of the CHT method and the electron beam deflection due to instrument and environmental instabilities. To separate these two effects, we also applied TMM to detect the position of the uniform diffraction disk. Because the disk is uniform in intensity for all patterns, TMM does not suffer from the issues as discussed in Section 4.2, and thus, it is can be used to detect the disk position accurately in this case. TMM is used as the reference for examining the error of CHT, as shown in Fig. 10a. At a fixed beam convergence angle of 0.8 mrad with the SNR kept at 280, the disk radius is proportional to camera length. The detection error plotted as function of the camera length L in Fig. 10b can be approximately fitted with , where and are the intercept and slope of the linear fit. The strain measurement precision is then given by for . The upper limit is determined by the detector size, which has to record enough diffraction disks in order to measure the reciprocal lattice. The precision improves as L increases. This improvement was confirmed by a calibration experiment performed on the unstrained region of our FinFET sample similar to the one in Section 4.4 using a CCD of 2048 by 2048 pixels with the camera length increased to the maximum allowed for keeping all nine disks for strain calculation (see Fig. 3). The strain precision estimated by the standard deviation is 0.030% along [110] direction and 0.031% along [001] direction, compared with the 0.036% along [110] direction and 0.076% along [001] direction reported in Section 4.4 using a detector of 1024 by 1024 pixels. At a fixed camera length, the diffraction disk radius increases as the beam convergence angle increases. Fig. 10c shows the increase in the CHT detection error as the convergence angle of the electron probe increases. Both camera length and SNR were kept constant at 360 mm and 150 in this case. Under these conditions, at the radius of 90 pixels, the beam semi-convergence angle is 1.6 mrad. Thus, the strain measurement precision decreases as the convergence angle increases using CHT, and the probe size and strain precision are competing factors. In other words, the convergence angle should be chosen as small as needed for the required spatial resolution. The minimum number of circular points for CHT is ~10. 4.6. Strain effect on the diffraction disk shape

Fig. 11. Interference effect on the diffraction disk shape without an abrupt interface. (a) Experimental strain profiles extracted from Figs. 4c and d along the dash-dotted line in Fig. 4b. The (-2-20) diffraction disk taken at the probe position of (b) P1 and (c) P2. (d) Strain profiles of a strained Si model for simulation with . The simulated (-2-20) diffraction disk at the probe position of (e) P3 and (f) P4 using the multislice method, showing the same feature as in (b) and (c). The center disk of the diffraction pattern is on the right side to the displayed disks.

Fig. 11 examines the effect of strain on the diffraction disk edge intensity. The change in the edge intensity is observed for the diffraction patterns taken at the positions P1 and P2 in Fig. 4b, in the form of bright and dark rings at one side of the diffracted disk. To understand the origin of this effect, we simulated electron nanodiffraction from a Si crystal model with a sinusoidal strain field along [110] direction. The model strain profile is plotted in Fig. 11d, which was designed to replicate the experimental strain distribution (Fig. 11a) along the dash-dotted line connecting P1 and P2 in Fig. 4b. Diffraction patterns simulated from P3 to P4 in the model using the same convergence angle as in experiment show similar ring effect at the edge of diffraction disks, as can be seen in the simulated (-2-20) disk at the P3 and P4 probe positions (Figs. 11e and f).

Fig. 12. Mechanism of interference effect in diffraction disks. (a) The distribution of amplitude and phase in the electron probe used for multislice simulation in Fig. 11. (b) Schematic diagram of convergent beam diffraction at a local strain minimum.

Next, we consider the complex wave function of the electron probe. Fig. 12a shows the line profiles for the amplitude and phase of the complex wave function across the probe center. The amplitude profile shows the characteristic primary peak at the center and the much smaller secondary peaks on both sides, while the phase increases by for each secondary peak. Because of the change in phase, contributions from the secondary peaks cancel each other to a good approximation when the sample illuminated by the primary and secondary peaks are the same. For a probe illuminated over a strained structure with a large strain gradient, the structures beneath the primary and secondary peaks have different lattice constants. As a first-order approximation, we only consider the largest secondary peak in the electron probe, which is in antiphase with the primary peak (Fig. 12a), while ignoring the effects of other secondary peaks. The ring effect is explained schematically in Fig. 12b. The ray paths of the direct and diffracted beams from the primary and secondary peaks are illustrated in colors (orange and blue). The average lattice constants differ at the sample regions illuminated by the primary and the secondary peak. The destructive interference between the two paths at the overlapping areas lowers the intensity in the diffracted beams and results in a bright edge where the interference is absent. The brighter edge, which is only obvious on one side of the disk (Fig. 11), is due to the fact that the diffraction of the primary peak contributes more in intensity than the secondary

peak. Therefore, the position of the bright edge provides information about the local strain environment. In Figs. 11b and e, the bright edge is away from the central beam, and the probe is at a strain minimum. On the other hand, in Figs. 11c and f, the bright edge is close to the center beam, as the probe is at a strain maximum. The change in edge intensity impacts the strain measurement accuracy dependent on the detection method, and the impact in the case of CHT is small from the same benefit of edge detection as discussed before.

Fig. 13. Interference effect on the diffraction disk shape with an abrupt strained interface. (a) The cross-section of the strained silicon model used for simulation, where the lattice constants differ by 3% for the left and right side of the model. The strained lattice is allowed to relax and the resulted lattice distortion is exaggerated in the figure for a better view. (b-d) The simulated (-220) diffraction disks at small lattice spacing region, interface, and large lattice spacing region, respectively. The center disk of the diffraction pattern is on the right side to the displayed disks.

Next, we consider electron nanodiffraction at an abrupt interface of two different crystal lattices. For this purpose, we built a Si crystal model of 8 nm in thickness with half of the structure unstrained, while the other half has a 3% tensile strain. The elastic relaxation is applied to mimic the real thin-film sample [37]. The cross-section of the model is illustrated in Fig. 13a with the exaggerated lattice distortion. Electron nanodiffraction was simulated at the same conditions as the previous case of continuous strain. The (-2-20) diffraction disks from unstrained region, interfacial region, and 3% strained region are shown in Figs. 13b, c, and d, respectively. Severe disk distortion is observed at the interface (Fig. 13c). The oval distortion is due to the overlapping of two disks originated from differently strained regions, which is similar to the selected area electron diffraction over a region with two different lattice spacings. This effect was also observed previously by Mahr et al [30]. The elastic relaxation used in our simulation makes the strain variation relatively smooth near the interface, which leads to bright edges and dark rings similar to Fig. 11 as well. The CHT measures the center of the oval disk and thus the average d-spacing under the electron probe. By detecting the weak, secondary edges, it is possible to separate the lattices on the two sides of the interface [30].

5. Conclusion We have developed a strategy for high resolution strain mapping based on SEND. The key to achieve high measurement precision in strained samples, while pushing for high spatial resolution using a convergent beam, is to develop an intensity insensitive method for diffraction disk detection. A method using circular Hough transform to detect the diffraction disks is described here. A weighted 2D lattice fitting is designed to calculate the deformation matrix and strain, from the detected disk positions. The method is applied to measure strain in a FinFET device at the spatial resolution of 1 nm. The effect of sample orientation, thickness, and strain field distribution on the strain measurement accuracy are examined based on the multislice simulations. The strain measurement precision is estimated by a calibration experiment on an unstrained region of the sample, as well as analytically from the diffraction patterns directly. Different experimental conditions are explored to provide a guideline for the optimal strain measurement strategy: signal-to-noise ratio of the diffraction pattern should be larger than 100 and camera length should be as large as there are enough diffraction disks to calculate the deformation matrix. Finally, we pointed out the difference in diffraction from the uniformly strained and non-uniformly strained regions. Together, our results show that SEND is a powerful technique to measure strain from crystalline materials at nanoscale, but the proper analysis is critical to achieve both high spatial resolution and high strain measurement precision.

Acknowledgments This work is supported by Intel Corporation through an SRC project.

References [1] T. Ghani et al., “A 90nm High Volume Manufacturing Logic Technology Featuring Novel 45nm Gate Length Strained Silicon CMOS Transistors,” IEDM, pp. 978–980, 2003. [2]

S. E. Thompson et al., “A 90-nm Logic Technology Featuring Strained-Silicon,” IEEE Trans. Electron Devices, vol. 51, no. 11, pp. 1790–1797, 2004.

[3]

P. B. Hirsch, Electron microscopy of thin crystals. Plenum Press, 1967.

[4]

M. J. Hytch, E. Snoeck, and R. Kilaas, “Quantitative measurement of displacement and strain fields from HREM micrographs,” Ultramicroscopy, vol. 74, pp. 131–146, 1998.

[5]

J. L. Rouviere and E. Sarigiannidou, “Theoretical discussions on the geometrical phase analysis,” Ultramicroscopy, vol. 106, pp. 1–17, 2005.

[6]

S. Kim et al., “Scanning moiré fringe imaging for quantitative strain mapping in semiconductor devices in semiconductor devices,” Appl. Phys. Lett., vol. 102, p. 161604, 2013.

[7]

F. H. Baumann, “High precision two-dimensional strain mapping in semiconductor devices using nanobeam electron diffraction in the transmission electron microscope,” Appl. Phys. Lett., vol. 104, no. 26, 2014.

[8]

M. J. Hÿtch and A. M. Minor, “Observing and measuring strain in nanostructures and devices with transmission electron microscopy,” MRS Bull., vol. 39, pp. 138–146, 2019.

[9]

A. D. Krawitz and T. M. Holden, “The Measurement of Residual Stresses Using Neutron Diffraction,” MRS Bull., vol. 15, no. 11, pp. 57–64, 1990.

[10] B. E. Warren, X-ray Diffraction. Courier Corporation, 1990. [11] J. Keckes et al., “X-ray nanodiffraction reveals strain and microstructure evolution in nanocrystalline thin films,” Scr. Mater., vol. 67, no. 9, pp. 748–751, 2012. [12] V. Senez et al., “Strain determination in silicon microstructures by combined convergent beam electron diffraction , process simulation , and micro-Raman spectroscopy,” J. Appl. Phys., vol. 94, p. 5574, 2003. [13] L. Jones et al., “Optimising multi-frame ADF-STEM for high-precision atomic-resolution strain mapping,” Ultramicroscopy, vol. 179, pp. 57–62, 2017. [14] J. M. Zuo, A. B. Shah, H. Kim, Y. Meng, W. Gao, and J. L. Rouviére, “Lattice and strain analysis of atomic resolution Z-contrast images based on template matching,” Ultramicroscopy, vol. 136, pp. 50–60, 2014. [15] A. B. Yankovich et al., “Picometre-precision analysis of scanning transmission electron microscopy images of platinum nanocatalysts,” Nat. Commun., vol. 5, no. May, pp. 1–7, 2014. [16] J.-M. Zuo, “Automated lattice parameter measurement from HOLZ lines and their use for the measurement of oxygen content in YBa2Cu3O7-δfrom nanometer-sized region,” Ultramicroscopy, vol. 41, no. 1–3, pp. 211–223, 1992. [17] J. Zuo, M. Kim, and R. Holmestad, “A new approach to lattice parameter measurements using dynamic electron diffraction and pattern matching,” J. Electron Microsc. (Tokyo)., vol. 47, no. 2, pp. 121–127, 1998. [18] A. Beche, J. L. Rouv re, L. C ment, and J. M. Hartmann, “Improved precision in strain measurement using nanobeam electron diffraction,” Appl. Phys. Lett., vol. 95, no. 12, 2009. [19] F. Uesugi, A. Hokazono, and S. Takeno, “Evaluation of two-dimensional strain distribution by STEM/NBD,” Ultramicroscopy, vol. 111, no. 8, pp. 995–998, 2011. [20] K. Müller-Caspary, A. Rosenauer, M. Schowalter, J. Zweck, R. Fritz, and K. Volz, “Strain measurement in semiconductor heterostructures by scanning transmission electron microscopy,” Microsc Microanal, vol. 18, no. 5, pp. 995–1009, 2012. [21] V. B. Ozdol et al., “Strain mapping at nanometer resolution using advanced nano-beam electron diffraction,” Appl. Phys. Lett., vol. 106, no. 25, 2015. [22] D. Cooper, T. Denneulin, N. Bernier, A. Béché, and J. L. Rouvière, “Strain mapping of semiconductor specimens with nm-scale resolution in a transmission electron

microscope,” Micron, vol. 80, pp. 145–165, 2016. [23] J. M. Zuo and J. C. H. Spence, Advanced Transmission Electron Microscopy. 2015. [24] J. M. Cowley, “Electron nanodiffraction: Progress and prospects,” J. Electron Microsc. (Tokyo)., vol. 45, no. 1, pp. 3–10, 1996. [25] J. Tao et al., “Direct imaging of nanoscale phase separation in La0.55Ca0.45MnO3: Relationship to colossal magnetoresistance,” Phys. Rev. Lett., vol. 103, no. 9, pp. 1–4, 2009. [26] J. Zuo and J. Tao, “Scanning Electron Nanodiffraction and Diffraction Imaging,” in Scanning Transmission Electron Microscopy, 2011, pp. 393–427. [27] P. A. Midgley and A. S. Eggeman, “Precession electron diffraction - A topical review,” IUCrJ, vol. 2, pp. 126–136, 2015. [28] K. Kim, H. Xing, J. Zuo, P. Zhang, and H. Wang, “TEM based high resolution and lowdose scanning electron nanodiffraction technique for nanostructure imaging and analysis,” Micron, vol. 71, pp. 39–45, 2015. [29] J. L. Rouviere, A. Béché, Y. Martin, T. Denneulin, and D. Cooper, “Improved strain precision with high spatial resolution using nanobeam precession electron diffraction,” Appl. Phys. Lett., vol. 103, no. 24, 2013. [30] C. Mahr et al., “Theoretical study of precision and accuracy of strain analysis by nanobeam electron diffraction,” Ultramicroscopy, vol. 158, pp. 38–48, 2015. [31] T. C. Pekin, C. Gammer, J. Ciston, A. M. Minor, and C. Ophus, “Optimizing disk registration algorithms for nanobeam electron diffraction strain mapping,” Ultramicroscopy, vol. 176, no. December 2016, pp. 170–176, 2017. [32] R. Yuan, Y. Meng, J. Zhang, and J.-M. Zuo, “Accurate Diffraction Peak Identification for Scanning Electron Nanodiffraction Based on Automated Image Processing and Feature Detection,” Microsc. Microanal., vol. 23, no. S1, pp. 180–181, 2017. [33] H. K. Yuen, J. Princen, J. Illingworth, and J. Kittler, “Comparative study of Hough Transform methods for circle finding,” Image Vis. Comput., vol. 8, no. 1, pp. 71–77, 1990. [34] T. J. Atherton and D. J. Kerbyson, “Size invariant circle detection,” Image Vis. Comput., vol. 17, pp. 795–803, 1999. [35] J. T. McKeown and J. C. H. Spence, “The kinematic convergent-beam electron diffraction method for nanocrystal structure determination,” J. Appl. Phys., vol. 106, p. 074309, 2009. [36] J. Spence, John; Zuo, Electron Microdiffraction, vol. 46, no. C. 1978. [37] J. M. Gibson and M. M. J. Treacy, “The effect of elastic relaxation on the local structure of lattice-modulated thin films,” Ultramicroscopy, vol. 14, no. 4, pp. 345–349, 1984.

Copyright © 2021 COEK.INFO. All rights reserved.